#------------------------------------------------------------------------------
#$Date: 2023-03-05 22:51:16 +0200 (Sun, 05 Mar 2023) $
#$Revision: 281633 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/85/1568598.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1568598
loop_
_publ_author_name
'Mauro, Daniela'
'Biagioni, Cristian'
_publ_section_title
;
 New Crystal-Structure Data on Bohuslavite,
 Fe3+4(PO4)3(SO4)(OH)(H2O)10·nH2O
;
_journal_issue                   2
_journal_name_full               Minerals
_journal_page_first              286
_journal_paper_doi               10.3390/min13020286
_journal_volume                  13
_journal_year                    2023
_chemical_compound_source        'Buca della Vena mine, Italy'
_chemical_formula_sum            'Fe16 O128 P12 S4'
_chemical_formula_weight         3441.48
_chemical_name_mineral           bohuslavite
_space_group_crystal_system      triclinic
_space_group_IT_number           1
_space_group_name_Hall           'P 1'
_space_group_name_H-M_alt        'P 1'
_audit_creation_method           SHELXL-2018/1
_cell_angle_alpha                92.345(6)
_cell_angle_beta                 90.153(8)
_cell_angle_gamma                120.34(3)
_cell_formula_units_Z            1
_cell_length_a                   13.3722(15)
_cell_length_b                   13.3488(18)
_cell_length_c                   21.585(3)
_cell_measurement_reflns_used    9463
_cell_measurement_temperature    303(2)
_cell_measurement_theta_max      27.53
_cell_measurement_theta_min      2.525
_cell_volume                     3321.3(13)
_computing_cell_refinement       'Apex4 (Bruker AXS Inc., 2022)'
_computing_data_collection       'Apex4 (Bruker AXS Inc., 2022)'
_computing_data_reduction        'Apex4 (Bruker AXS Inc., 2022)'
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      303(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.968
_diffrn_measurement_device_type  'Bruker D8 Venture'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0726
_diffrn_reflns_av_unetI/netI     0.0761
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.968
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            107166
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.968
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.862
_diffrn_reflns_theta_min         1.977
_diffrn_source                   micro-focus
_exptl_absorpt_coefficient_mu    2.019
_exptl_absorpt_correction_T_max  0.957
_exptl_absorpt_correction_T_min  0.808
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_crystal_colour            lilac
_exptl_crystal_density_diffrn    1.721
_exptl_crystal_density_meas      ?
_exptl_crystal_description       'tabular pseudo-hexagonal'
_exptl_crystal_F_000             1684
_exptl_crystal_size_max          0.060
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.010
_refine_diff_density_max         4.688
_refine_diff_density_min         -2.040
_refine_diff_density_rms         0.382
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.47(6)
_refine_ls_extinction_coef       0.028(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/1 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.089
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     773
_refine_ls_number_reflns         29739
_refine_ls_number_restraints     67
_refine_ls_restrained_S_all      1.088
_refine_ls_R_factor_all          0.1968
_refine_ls_R_factor_gt           0.1498
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.2468P)²+55.8200P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.4013
_refine_ls_wR_factor_ref         0.4527
_reflns_Friedel_coverage         1.000
_reflns_Friedel_fraction_full    0.997
_reflns_Friedel_fraction_max     0.968
_reflns_number_gt                19578
_reflns_number_total             29739
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            minerals-2210187-supplementary.cif
_cod_data_source_block           shelx
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_crystal_density_meas' value 'not measured' was
changed to '?' -- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 
;
_cod_original_cell_volume        3321.2(11)
_cod_database_code               1568598
_shelx_shelxl_version_number     2018/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe11 Fe -0.8693(3) -1.8828(3) 0.3645(2) 0.0368(10) Uani 1 1 d . . . . .
Fe21 Fe -0.6489(3) -1.6794(2) 0.1860(2) 0.0369(10) Uani 1 1 d . . . . .
Fe31 Fe 0.1193(3) -1.1375(2) 0.1904(2) 0.0376(6) Uani 1 1 d . . . . .
Fe41 Fe -0.3145(3) -1.2271(3) 0.3283(2) 0.0376(6) Uani 1 1 d . . . . .
Fe51 Fe -0.1114(3) -0.9145(3) 0.1867(2) 0.0379(10) Uani 1 1 d . . . . .
Fe61 Fe -0.5418(3) -1.9986(3) 0.3302(2) 0.0374(10) Uani 1 1 d . . . . .
Fe71 Fe -0.7673(3) -1.4598(2) 0.3278(2) 0.0376(6) Uani 1 1 d . . . . .
Fe81 Fe -0.5514(3) -1.2373(3) 0.1518(2) 0.0368(10) Uani 1 1 d . . . . .
P11 P -0.8773(4) -1.7151(4) 0.2559(4) 0.0361(6) Uani 1 1 d D . . . .
P21 P -0.3597(4) -1.0454(4) 0.2556(4) 0.0361(6) Uani 1 1 d D . . . .
P31 P -0.6951(4) -1.8984(4) 0.2646(4) 0.0361(6) Uani 1 1 d D . . . .
P41 P -0.7305(4) -1.2362(4) 0.2574(4) 0.0361(6) Uani 1 1 d D . . . .
P51 P -0.0568(4) -1.0834(4) 0.2655(4) 0.0361(6) Uani 1 1 d D . . . .
P61 P -0.5422(4) -1.4134(4) 0.2496(4) 0.0361(6) Uani 1 1 d D . . . .
S11 S -0.4725(7) -1.0266(7) 0.0548(5) 0.062(2) Uani 1 1 d D . . . .
S21 S -0.6427(7) -1.7314(6) 0.4599(5) 0.063(2) Uani 1 1 d D . . . .
O1 O -0.735(2) -1.545(2) 0.3969(10) 0.056(5) Uiso 1 1 d . . . . .
O2 O -0.7558(16) -1.9122(17) 0.3254(7) 0.039(4) Uiso 1 1 d D . . . .
O3 O -0.0090(18) -1.0174(18) 0.3272(8) 0.045(5) Uiso 1 1 d D . . . .
O4 O -0.990(2) -1.865(2) 0.4184(10) 0.056(5) Uiso 1 1 d . . . . .
O5 O -0.8621(19) -1.7650(18) 0.3147(8) 0.046(5) Uiso 1 1 d D . . . .
O6 O -0.739(2) -1.750(2) 0.4180(11) 0.064(6) Uiso 1 1 d D . . . .
O7 O -0.874(2) -1.995(2) 0.4339(12) 0.064(6) Uiso 1 1 d . . . . .
O8 O -0.8123(16) -1.7262(17) 0.1989(8) 0.040(4) Uiso 1 1 d D . . . .
O9 O -0.6318(17) -1.7708(14) 0.2494(8) 0.039(4) Uiso 1 1 d D . . . .
O10 O -0.5779(18) -1.5418(14) 0.2429(9) 0.040(4) Uiso 1 1 d D . . . .
O11 O -0.719(2) -1.814(2) 0.1209(12) 0.064(6) Uiso 1 1 d . . . . .
O12 O -0.493(2) -1.641(3) 0.1498(12) 0.066(6) Uiso 1 1 d . . . . .
O13 O -0.660(3) -1.589(3) 0.1120(13) 0.073(7) Uiso 1 1 d . . . . .
O14 O 0.0008(19) -1.1536(19) 0.2460(10) 0.047(5) Uiso 1 1 d D . . . .
O15 O -0.8184(16) -1.1979(17) 0.2510(9) 0.042(4) Uiso 1 1 d D . . . .
O16 O -0.1847(13) -1.1710(15) 0.2727(8) 0.035(4) Uiso 1 1 d D . . . .
O17 O -0.7824(18) -1.9698(18) 0.2114(8) 0.047(5) Uiso 1 1 d D . . . .
O18 O 0.004(3) -1.305(3) 0.1558(13) 0.076(8) Uiso 1 1 d . . . . .
O19 O -0.3680(19) -1.1193(17) 0.3102(8) 0.045(5) Uiso 1 1 d D . . . .
O20 O -0.206(3) -1.113(3) 0.3993(13) 0.071(7) Uiso 1 1 d . . . . .
O21 O -0.438(2) -1.279(2) 0.3931(10) 0.051(5) Uiso 1 1 d . . . . .
O22 O 0.229(2) -1.130(2) 0.1240(11) 0.060(6) Uiso 1 1 d . . . . .
O23 O -0.958(2) -2.087(2) 0.1237(11) 0.055(5) Uiso 1 1 d . . . . .
O24 O -0.4150(13) -1.3503(15) 0.2662(8) 0.035(4) Uiso 1 1 d D . . . .
O25 O -0.265(2) -1.343(2) 0.3595(11) 0.064(6) Uiso 1 1 d . . . . .
O26 O -1.0070(14) -1.7779(17) 0.2362(9) 0.041(4) Uiso 1 1 d D . . . .
O27 O -0.2333(14) -0.9583(16) 0.2448(9) 0.038(4) Uiso 1 1 d D . . . .
O28 O -0.215(2) -1.048(2) 0.1264(11) 0.059(6) Uiso 1 1 d . . . . .
O29 O -0.990(3) -1.875(3) 0.1185(13) 0.066(7) Uiso 1 1 d . . . . .
O30 O -0.6461(17) -1.1612(17) 0.3111(8) 0.043(4) Uiso 1 1 d D . . . .
O31 O -0.4208(14) -0.9780(13) 0.2748(7) 0.027(3) Uiso 1 1 d D . . . .
O32 O -0.8370(17) -1.5875(13) 0.2690(8) 0.036(4) Uiso 1 1 d D . . . .
O33 O -0.6087(18) -1.3933(19) 0.3005(9) 0.048(5) Uiso 1 1 d D . . . .
O34 O -0.926(3) -1.503(3) 0.3640(13) 0.074(7) Uiso 1 1 d . . . . .
O35 O -0.696(3) -1.327(3) 0.3959(13) 0.074(8) Uiso 1 1 d . . . . .
O36 O -0.6658(19) -1.223(2) 0.1976(8) 0.047(5) Uiso 1 1 d D . . . .
O37 O -0.4177(18) -1.1224(17) 0.1979(8) 0.044(5) Uiso 1 1 d D . . . .
O38 O -0.682(2) -1.357(2) 0.0910(11) 0.059(6) Uiso 1 1 d . . . . .
O39 O -0.5474(18) -1.1132(18) 0.0983(9) 0.052(5) Uiso 1 1 d D . . . .
O40 O -0.0399(18) -1.0025(16) 0.2146(8) 0.042(4) Uiso 1 1 d D . . . .
O41 O -0.166(2) -0.818(2) 0.1377(11) 0.058(5) Uiso 1 1 d . . . . .
O42 O -0.6027(16) -1.9330(17) 0.2756(9) 0.040(4) Uiso 1 1 d D . . . .
O43 O -0.427(2) -1.828(2) 0.3699(10) 0.054(5) Uiso 1 1 d . . . . .
O44 O -0.484(2) -2.062(2) 0.3989(10) 0.051(5) Uiso 1 1 d . . . . .
O45 O -0.659(3) -2.010(3) 0.3952(14) 0.075(8) Uiso 1 1 d . . . . .
O46 O -0.7960(16) -1.3627(14) 0.2765(8) 0.038(4) Uiso 1 1 d D . . . .
O47 O -0.447(2) -1.253(2) 0.0892(11) 0.062(6) Uiso 1 1 d . . . . .
O48 O -0.569(2) -1.374(2) 0.1893(9) 0.054(5) Uiso 1 1 d D . . . .
O49 O -0.536(3) -0.990(4) 0.0132(15) 0.107(11) Uiso 1 1 d D . . . .
O50 O -0.416(3) -1.076(3) 0.0154(13) 0.079(8) Uiso 1 1 d D . . . .
O51 O -0.381(3) -0.921(2) 0.0904(14) 0.091(9) Uiso 1 1 d D . . . .
O52 O -0.692(2) -1.8380(19) 0.4969(11) 0.066(6) Uiso 1 1 d D . . . .
O53 O -0.548(2) -1.726(3) 0.4220(12) 0.078(8) Uiso 1 1 d D . . . .
O54 O -0.601(3) -1.625(2) 0.4999(13) 0.086(8) Uiso 1 1 d D . . . .
Fe12 Fe -0.8075(7) -0.8887(5) 0.8659(3) 0.0780(18) Uani 1 1 d . . . . .
Fe22 Fe -0.5919(7) -1.6669(5) 0.6894(3) 0.0803(18) Uani 1 1 d . . . . .
Fe32 Fe -0.8213(7) -1.1291(5) 0.6868(3) 0.0813(19) Uani 1 1 d . . . . .
Fe42 Fe -0.2530(6) -1.2148(6) 0.8312(3) 0.0778(17) Uani 1 1 d . . . . .
Fe52 Fe -1.0480(6) -0.9008(5) 0.6890(3) 0.0773(17) Uani 1 1 d . . . . .
Fe62 Fe -0.4915(6) -1.2420(5) 0.6528(3) 0.0765(17) Uani 1 1 d . . . . .
Fe72 Fe -0.7099(6) -1.4494(5) 0.8317(3) 0.0771(17) Uani 1 1 d . . . . .
Fe82 Fe -0.4814(7) -0.9917(6) 0.8274(3) 0.0827(18) Uani 1 1 d . . . . .
P12 P -0.6710(12) -1.2318(9) 0.7526(5) 0.078(3) Uani 1 1 d D . . . .
P22 P -0.3012(12) -1.0421(10) 0.7511(5) 0.081(3) Uani 1 1 d D . . . .
P32 P -0.9996(12) -1.0799(10) 0.7624(5) 0.078(3) Uani 1 1 d D . . . .
P42 P -0.4838(12) -1.4105(10) 0.7617(5) 0.081(3) Uani 1 1 d D . . . .
P52 P -0.6313(11) -0.8935(9) 0.7610(5) 0.073(3) Uani 1 1 d D . . . .
P62 P -0.8201(12) -0.7131(9) 0.7679(5) 0.081(3) Uani 1 1 d D . . . .
S12 S -0.7174(8) -1.3929(8) 0.5550(5) 0.070(2) Uani 1 1 d D . . . .
S22 S -0.8875(9) -1.1026(9) 0.9646(5) 0.072(3) Uani 1 1 d D . . . .
O55 O -0.755(2) -1.188(3) 0.7467(13) 0.069(7) Uiso 1 1 d D . . . .
O56 O -0.702(3) -0.914(3) 0.8191(13) 0.095(10) Uiso 1 1 d D . . . .
O57 O -0.567(3) -0.766(2) 0.7439(15) 0.086(9) Uiso 1 1 d D . . . .
O58 O -0.953(3) -1.001(3) 0.8212(12) 0.092(9) Uiso 1 1 d D . . . .
O59 O -0.809(2) -1.006(2) 0.9253(12) 0.077(7) Uiso 1 1 d D . . . .
O60 O -0.916(3) -0.881(3) 0.9349(14) 0.083(8) Uiso 1 1 d . . . . .
O61 O -0.666(3) -0.772(3) 0.9256(14) 0.081(8) Uiso 1 1 d . . . . .
O62 O -0.523(3) -1.537(2) 0.7469(15) 0.082(8) Uiso 1 1 d D . . . .
O63 O -0.436(4) -1.600(4) 0.649(2) 0.135(16) Uiso 1 1 d . . . . .
O64 O -0.756(3) -0.727(3) 0.7124(13) 0.092(9) Uiso 1 1 d D . . . .
O65 O -0.589(4) -1.566(4) 0.6238(17) 0.113(12) Uiso 1 1 d . . . . .
O66 O -0.660(3) -0.803(3) 0.6255(15) 0.085(9) Uiso 1 1 d . . . . .
O67 O -0.931(4) -1.140(4) 0.744(2) 0.137(15) Uiso 1 1 d D . . . .
O68 O -0.716(2) -0.966(3) 0.7086(12) 0.080(8) Uiso 1 1 d D . . . .
O69 O -0.883(3) -1.068(3) 0.6212(17) 0.098(10) Uiso 1 1 d . . . . .
O70 O -0.912(4) -1.282(4) 0.6378(17) 0.109(11) Uiso 1 1 d . . . . .
O71 O -0.702(3) -1.116(3) 0.6197(17) 0.096(10) Uiso 1 1 d . . . . .
O72 O -0.354(2) -1.351(3) 0.7839(16) 0.093(9) Uiso 1 1 d D . . . .
O73 O -0.787(3) -0.587(2) 0.7769(14) 0.079(8) Uiso 1 1 d D . . . .
O74 O -0.196(4) -1.309(4) 0.877(2) 0.121(13) Uiso 1 1 d . . . . .
O75 O -0.325(3) -1.129(3) 0.8022(13) 0.085(8) Uiso 1 1 d D . . . .
O76 O -1.134(3) -1.071(3) 0.8900(16) 0.094(10) Uiso 1 1 d . . . . .
O77 O -0.376(3) -1.256(3) 0.9014(15) 0.081(8) Uiso 1 1 d . . . . .
O78 O -0.170(2) -0.969(3) 0.7443(14) 0.084(8) Uiso 1 1 d D . . . .
O79 O -0.946(2) -0.786(3) 0.7464(16) 0.096(10) Uiso 1 1 d D . . . .
O80 O -1.162(3) -1.010(3) 0.6214(14) 0.080(8) Uiso 1 1 d . . . . .
O81 O -0.997(3) -1.011(3) 0.7069(13) 0.093(9) Uiso 1 1 d D . . . .
O82 O -0.918(3) -0.837(3) 0.6205(15) 0.086(9) Uiso 1 1 d . . . . .
O83 O -1.076(3) -0.773(3) 0.6508(15) 0.089(9) Uiso 1 1 d . . . . .
O84 O -0.364(3) -1.115(3) 0.6918(11) 0.078(8) Uiso 1 1 d D . . . .
O85 O -0.512(3) -1.358(3) 0.7075(13) 0.091(9) Uiso 1 1 d D . . . .
O86 O -0.589(3) -1.199(4) 0.6978(16) 0.124(14) Uiso 1 1 d D . . . .
O87 O -0.390(3) -1.276(3) 0.5968(15) 0.087(9) Uiso 1 1 d . . . . .
O88 O -0.482(3) -1.142(3) 0.5837(16) 0.092(9) Uiso 1 1 d . . . . .
O89 O -0.618(2) -1.371(2) 0.5950(11) 0.067(6) Uiso 1 1 d D . . . .
O90 O -0.556(3) -1.400(3) 0.8117(13) 0.092(9) Uiso 1 1 d D . . . .
O91 O -1.126(2) -1.167(2) 0.7758(14) 0.076(7) Uiso 1 1 d D . . . .
O92 O -0.731(3) -1.355(2) 0.7745(14) 0.080(8) Uiso 1 1 d D . . . .
O93 O -0.719(3) -1.551(3) 0.9008(15) 0.088(9) Uiso 1 1 d . . . . .
O94 O -0.632(3) -1.303(3) 0.8938(14) 0.080(8) Uiso 1 1 d . . . . .
O95 O -0.885(3) -1.493(3) 0.8627(16) 0.094(10) Uiso 1 1 d . . . . .
O96 O -0.544(2) -0.931(2) 0.7745(12) 0.065(6) Uiso 1 1 d D . . . .
O97 O -0.594(3) -1.150(3) 0.8065(13) 0.086(9) Uiso 1 1 d D . . . .
O98 O -0.356(3) -0.972(3) 0.7737(14) 0.079(8) Uiso 1 1 d D . . . .
O99 O -0.415(4) -1.044(4) 0.8925(18) 0.104(11) Uiso 1 1 d . . . . .
O100 O -0.387(4) -0.827(4) 0.8685(19) 0.112(12) Uiso 1 1 d . . . . .
O101 O -0.603(3) -1.019(3) 0.8950(15) 0.086(9) Uiso 1 1 d . . . . .
O102 O -0.796(3) -0.760(3) 0.8269(12) 0.081(8) Uiso 1 1 d D . . . .
O103 O -0.743(3) -1.495(2) 0.5147(12) 0.078(7) Uiso 1 1 d D . . . .
O104 O -0.686(3) -1.301(3) 0.5113(14) 0.094(9) Uiso 1 1 d D . . . .
O105 O -0.825(2) -1.412(3) 0.5853(15) 0.094(9) Uiso 1 1 d D . . . .
O106 O -0.812(2) -1.127(3) 1.0020(12) 0.079(8) Uiso 1 1 d D . . . .
O107 O -0.966(3) -1.205(3) 0.9251(15) 0.096(10) Uiso 1 1 d D . . . .
O108 O -0.946(3) -1.057(4) 1.0049(16) 0.103(11) Uiso 1 1 d D . . . .
OW1 O -0.588(3) -0.826(3) 0.0283(15) 0.090(9) Uiso 1 1 d . . . . .
OW2 O -0.781(3) -1.314(3) -0.0069(16) 0.094(10) Uiso 1 1 d . . . . .
OW3 O -1.177(4) -0.961(4) 0.9853(19) 0.127(13) Uiso 1 1 d . . . . .
OW4 O -0.921(4) -0.719(4) 0.5294(17) 0.102(11) Uiso 1 1 d . . . . .
OW5 O 0.0689(19) -0.6386(19) 0.0233(9) 0.053(5) Uiso 1 1 d . . . . .
OW6 O -0.936(5) -1.483(5) 0.164(2) 0.160(18) Uiso 1 1 d . . . . .
OW7 O -0.319(8) -0.752(8) 0.981(4) 0.25(4) Uiso 1 1 d . . . . .
OW8 O -0.891(7) -1.299(7) 0.839(3) 0.20(3) Uiso 1 1 d . . . . .
OW9 O -0.781(3) -2.172(3) 0.4792(16) 0.107(10) Uiso 1 1 d . . . . .
OW10 O -1.009(5) -1.338(5) 0.334(2) 0.152(17) Uiso 1 1 d . . . . .
OW12 O -1.142(7) -1.395(7) 0.764(3) 0.22(3) Uiso 1 1 d . . . . .
OW13 O -0.252(4) -1.381(4) 0.1904(17) 0.115(11) Uiso 1 1 d . . . . .
OW14 O -0.114(3) -0.774(3) 0.3632(16) 0.107(10) Uiso 1 1 d . . . . .
OW15 O -0.421(3) -0.800(3) 0.1883(14) 0.090(9) Uiso 1 1 d . . . . .
OW16 O -0.432(3) -1.402(3) 0.4914(15) 0.087(9) Uiso 1 1 d . . . . .
OW17 O -0.433(2) -1.575(2) 0.3314(11) 0.069(6) Uiso 1 1 d . . . . .
OW18 O -0.346(7) -1.584(7) 0.538(3) 0.23(3) Uiso 1 1 d . . . . .
OW1A O -1.0897(18) -2.2838(18) 0.5006(9) 0.029(4) Uiso 0.72(3) 1 d . . P . .
OW1B O -1.202(5) -2.355(5) 0.478(2) 0.029(4) Uiso 0.28(3) 1 d . . P . .
OW3A O -1.258(2) -0.881(2) 0.5066(11) 0.050(6) Uiso 0.80(4) 1 d . . P . .
OW3B O -1.162(9) -0.793(9) 0.538(5) 0.050(6) Uiso 0.20(4) 1 d . . P . .
OW2A O -0.399(3) -1.474(3) 0.0089(14) 0.048(6) Uiso 0.61(3) 1 d . . P . .
OW2B O -0.424(4) -1.582(4) 0.036(2) 0.048(6) Uiso 0.39(3) 1 d . . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Fe11 O2 101.1(8) . . ?
O5 Fe11 O3 99.3(9) . 1_445 ?
O2 Fe11 O3 97.8(8) . 1_445 ?
O5 Fe11 O6 86.3(9) . . ?
O2 Fe11 O6 89.3(9) . . ?
O3 Fe11 O6 169.9(10) 1_445 . ?
O5 Fe11 O4 87.5(9) . . ?
O2 Fe11 O4 171.1(9) . . ?
O3 Fe11 O4 83.1(9) 1_445 . ?
O6 Fe11 O4 88.8(10) . . ?
O5 Fe11 O7 170.0(9) . . ?
O2 Fe11 O7 85.4(9) . . ?
O3 Fe11 O7 87.3(9) 1_445 . ?
O6 Fe11 O7 86.1(10) . . ?
O4 Fe11 O7 85.8(10) . . ?
O9 Fe21 O10 90.2(8) . . ?
O9 Fe21 O8 98.6(8) . . ?
O10 Fe21 O8 98.0(8) . . ?
O9 Fe21 O11 94.1(9) . . ?
O10 Fe21 O11 175.3(10) . . ?
O8 Fe21 O11 83.3(10) . . ?
O9 Fe21 O12 91.0(10) . . ?
O10 Fe21 O12 92.7(10) . . ?
O8 Fe21 O12 165.6(9) . . ?
O11 Fe21 O12 85.3(11) . . ?
O9 Fe21 O13 174.3(10) . . ?
O10 Fe21 O13 93.6(10) . . ?
O8 Fe21 O13 85.0(10) . . ?
O11 Fe21 O13 81.9(11) . . ?
O12 Fe21 O13 84.6(11) . . ?
O14 Fe31 O15 91.2(8) . 1_655 ?
O14 Fe31 O17 92.9(9) . 1_665 ?
O15 Fe31 O17 99.4(8) 1_655 1_665 ?
O14 Fe31 O22 173.2(10) . . ?
O15 Fe31 O22 93.5(9) 1_655 . ?
O17 Fe31 O22 91.1(10) 1_665 . ?
O14 Fe31 O18 87.5(11) . . ?
O15 Fe31 O18 90.6(11) 1_655 . ?
O17 Fe31 O18 169.9(11) 1_665 . ?
O22 Fe31 O18 87.5(11) . . ?
O14 Fe31 O23 88.1(9) . 1_665 ?
O15 Fe31 O23 175.3(9) 1_655 1_665 ?
O17 Fe31 O23 85.2(9) 1_665 1_665 ?
O22 Fe31 O23 86.9(10) . 1_665 ?
O18 Fe31 O23 84.7(11) . 1_665 ?
O16 Fe41 O19 99.1(8) . . ?
O16 Fe41 O24 90.6(7) . . ?
O19 Fe41 O24 96.7(8) . . ?
O16 Fe41 O21 174.5(8) . . ?
O19 Fe41 O21 82.9(9) . . ?
O24 Fe41 O21 94.2(8) . . ?
O16 Fe41 O20 90.6(9) . . ?
O19 Fe41 O20 90.0(10) . . ?
O24 Fe41 O20 172.9(10) . . ?
O21 Fe41 O20 84.2(10) . . ?
O16 Fe41 O25 87.5(9) . . ?
O19 Fe41 O25 172.4(9) . . ?
O24 Fe41 O25 87.0(9) . . ?
O21 Fe41 O25 90.2(10) . . ?
O20 Fe41 O25 86.1(11) . . ?
O26 Fe51 O27 92.5(8) 1_665 . ?
O26 Fe51 O40 93.3(8) 1_665 . ?
O27 Fe51 O40 101.1(8) . . ?
O26 Fe51 O28 173.7(9) 1_665 . ?
O27 Fe51 O28 92.1(9) . . ?
O40 Fe51 O28 90.0(9) . . ?
O26 Fe51 O29 91.9(10) 1_665 1_665 ?
O27 Fe51 O29 175.3(10) . 1_665 ?
O40 Fe51 O29 80.5(10) . 1_665 ?
O28 Fe51 O29 83.4(10) . 1_665 ?
O26 Fe51 O41 90.1(9) 1_665 . ?
O27 Fe51 O41 91.9(9) . . ?
O40 Fe51 O41 166.3(9) . . ?
O28 Fe51 O41 85.5(10) . . ?
O29 Fe51 O41 86.2(11) 1_665 . ?
O42 Fe61 O30 100.3(8) . 1_545 ?
O42 Fe61 O31 93.3(7) . 1_545 ?
O30 Fe61 O31 97.7(8) 1_545 1_545 ?
O42 Fe61 O45 89.3(11) . . ?
O30 Fe61 O45 86.4(11) 1_545 . ?
O31 Fe61 O45 174.6(10) 1_545 . ?
O42 Fe61 O44 172.5(9) . . ?
O30 Fe61 O44 82.5(9) 1_545 . ?
O31 Fe61 O44 93.2(8) 1_545 . ?
O45 Fe61 O44 83.8(11) . . ?
O42 Fe61 O43 88.9(9) . . ?
O30 Fe61 O43 168.6(9) 1_545 . ?
O31 Fe61 O43 88.4(8) 1_545 . ?
O45 Fe61 O43 86.9(11) . . ?
O44 Fe61 O43 87.6(9) . . ?
O32 Fe71 O46 92.8(8) . . ?
O32 Fe71 O33 97.6(8) . . ?
O46 Fe71 O33 92.3(9) . . ?
O32 Fe71 O35 176.7(11) . . ?
O46 Fe71 O35 89.5(10) . . ?
O33 Fe71 O35 84.6(10) . . ?
O32 Fe71 O34 91.6(10) . . ?
O46 Fe71 O34 84.0(10) . . ?
O33 Fe71 O34 170.3(10) . . ?
O35 Fe71 O34 86.3(12) . . ?
O32 Fe71 O1 96.9(8) . . ?
O46 Fe71 O1 169.5(9) . . ?
O33 Fe71 O1 90.4(9) . . ?
O35 Fe71 O1 80.6(11) . . ?
O34 Fe71 O1 91.7(10) . . ?
O37 Fe81 O36 98.0(9) . . ?
O37 Fe81 O48 98.8(9) . . ?
O36 Fe81 O48 98.0(10) . . ?
O37 Fe81 O47 89.6(9) . . ?
O36 Fe81 O47 169.4(10) . . ?
O48 Fe81 O47 88.0(10) . . ?
O37 Fe81 O39 90.6(9) . . ?
O36 Fe81 O39 85.4(9) . . ?
O48 Fe81 O39 169.4(9) . . ?
O47 Fe81 O39 87.2(10) . . ?
O37 Fe81 O38 172.1(9) . . ?
O36 Fe81 O38 88.9(10) . . ?
O48 Fe81 O38 83.9(10) . . ?
O47 Fe81 O38 83.0(10) . . ?
O39 Fe81 O38 86.1(10) . . ?
O5 P11 O32 108.9(11) . . ?
O5 P11 O26 109.8(12) . . ?
O32 P11 O26 107.9(11) . . ?
O5 P11 O8 115.3(11) . . ?
O32 P11 O8 108.5(11) . . ?
O26 P11 O8 106.2(11) . . ?
O37 P21 O27 111.1(12) . . ?
O37 P21 O31 110.6(11) . . ?
O27 P21 O31 108.3(10) . . ?
O37 P21 O19 110.4(12) . . ?
O27 P21 O19 109.4(12) . . ?
O31 P21 O19 106.9(11) . . ?
O2 P31 O9 109.1(11) . . ?
O2 P31 O17 111.2(12) . . ?
O9 P31 O17 108.8(12) . . ?
O2 P31 O42 106.4(12) . . ?
O9 P31 O42 107.5(11) . . ?
O17 P31 O42 113.8(12) . . ?
O15 P41 O36 111.4(13) . . ?
O15 P41 O46 107.2(11) . . ?
O36 P41 O46 112.0(12) . . ?
O15 P41 O30 107.1(12) . . ?
O36 P41 O30 110.9(12) . . ?
O46 P41 O30 108.0(12) . . ?
O40 P51 O3 111.5(12) . . ?
O40 P51 O16 110.9(11) . . ?
O3 P51 O16 108.1(12) . . ?
O40 P51 O14 107.9(12) . . ?
O3 P51 O14 112.0(12) . . ?
O16 P51 O14 106.4(12) . . ?
O24 P61 O33 110.4(12) . . ?
O24 P61 O48 112.7(12) . . ?
O33 P61 O48 107.7(13) . . ?
O24 P61 O10 105.1(11) . . ?
O33 P61 O10 110.8(12) . . ?
O48 P61 O10 110.2(13) . . ?
O39 S11 O50 108.8(17) . . ?
O39 S11 O49 113.4(19) . . ?
O50 S11 O49 108(2) . . ?
O39 S11 O51 109.3(17) . . ?
O50 S11 O51 109.3(19) . . ?
O49 S11 O51 108(2) . . ?
O54 S21 O53 110.8(18) . . ?
O54 S21 O6 111.4(18) . . ?
O53 S21 O6 108.7(17) . . ?
O54 S21 O52 111.8(17) . . ?
O53 S21 O52 109.1(17) . . ?
O6 S21 O52 104.8(16) . . ?
P31 O2 Fe11 141.0(12) . . ?
P51 O3 Fe11 140.9(14) . 1_665 ?
P11 O5 Fe11 155.8(14) . . ?
S21 O6 Fe11 138.5(18) . . ?
P11 O8 Fe21 132.7(11) . . ?
P31 O9 Fe21 135.5(12) . . ?
P61 O10 Fe21 143.8(13) . . ?
P51 O14 Fe31 137.1(14) . . ?
P41 O15 Fe31 141.1(12) . 1_455 ?
P51 O16 Fe41 145.1(12) . . ?
P31 O17 Fe31 134.0(13) . 1_445 ?
P21 O19 Fe41 136.0(13) . . ?
P61 O24 Fe41 134.8(11) . . ?
P11 O26 Fe51 136.3(13) . 1_445 ?
P21 O27 Fe51 143.7(13) . . ?
P41 O30 Fe61 136.7(13) . 1_565 ?
P21 O31 Fe61 136.8(10) . 1_565 ?
P11 O32 Fe71 146.0(12) . . ?
P61 O33 Fe71 139.1(13) . . ?
P41 O36 Fe81 149.9(15) . . ?
P21 O37 Fe81 151.9(14) . . ?
S11 O39 Fe81 140.6(15) . . ?
P51 O40 Fe51 137.4(13) . . ?
P31 O42 Fe61 146.7(13) . . ?
P41 O46 Fe71 137.4(12) . . ?
P61 O48 Fe81 141.2(15) . . ?
O102 Fe12 O56 100.7(15) . . ?
O102 Fe12 O58 93.6(14) . . ?
O56 Fe12 O58 99.4(15) . . ?
O102 Fe12 O59 167.6(13) . . ?
O56 Fe12 O59 86.0(14) . . ?
O58 Fe12 O59 95.5(13) . . ?
O102 Fe12 O60 92.3(14) . . ?
O56 Fe12 O60 165.9(14) . . ?
O58 Fe12 O60 85.3(13) . . ?
O59 Fe12 O60 80.3(12) . . ?
O102 Fe12 O61 88.7(13) . . ?
O56 Fe12 O61 88.2(15) . . ?
O58 Fe12 O61 171.5(13) . . ?
O59 Fe12 O61 81.0(12) . . ?
O60 Fe12 O61 86.4(12) . . ?
O62 Fe22 O57 93.4(13) . 1_545 ?
O62 Fe22 O65 90.3(15) . . ?
O57 Fe22 O65 167.6(16) 1_545 . ?
O62 Fe22 O64 97.5(14) . 1_545 ?
O57 Fe22 O64 94.9(14) 1_545 1_545 ?
O65 Fe22 O64 96.3(16) . 1_545 ?
O62 Fe22 O63 87.6(17) . . ?
O57 Fe22 O63 95.6(17) 1_545 . ?
O65 Fe22 O63 72.7(19) . . ?
O64 Fe22 O63 168.0(17) 1_545 . ?
O62 Fe22 O66 177.6(15) . 1_545 ?
O57 Fe22 O66 87.1(13) 1_545 1_545 ?
O65 Fe22 O66 88.7(15) . 1_545 ?
O64 Fe22 O66 84.8(13) 1_545 1_545 ?
O63 Fe22 O66 90.0(17) . 1_545 ?
O67 Fe32 O68 92.9(18) . . ?
O67 Fe32 O55 91.0(15) . . ?
O68 Fe32 O55 95.7(13) . . ?
O67 Fe32 O70 101.4(19) . . ?
O68 Fe32 O70 162.2(15) . . ?
O55 Fe32 O70 94.6(14) . . ?
O67 Fe32 O69 92.2(18) . . ?
O68 Fe32 O69 84.3(14) . . ?
O55 Fe32 O69 176.7(14) . . ?
O70 Fe32 O69 84.5(16) . . ?
O67 Fe32 O71 177.4(18) . . ?
O68 Fe32 O71 87.5(14) . . ?
O55 Fe32 O71 91.5(13) . . ?
O70 Fe32 O71 77.8(16) . . ?
O69 Fe32 O71 85.3(15) . . ?
O72 Fe42 O91 94.8(13) . 1_655 ?
O72 Fe42 O75 93.7(15) . . ?
O91 Fe42 O75 101.7(13) 1_655 . ?
O72 Fe42 O74 88.3(17) . . ?
O91 Fe42 O74 88.9(16) 1_655 . ?
O75 Fe42 O74 169.0(16) . . ?
O72 Fe42 O77 91.7(14) . . ?
O91 Fe42 O77 172.5(13) 1_655 . ?
O75 Fe42 O77 81.6(13) . . ?
O74 Fe42 O77 87.6(16) . . ?
O72 Fe42 O76 174.5(15) . 1_655 ?
O91 Fe42 O76 85.7(13) 1_655 1_655 ?
O75 Fe42 O76 91.5(14) . 1_655 ?
O74 Fe42 O76 86.2(16) . 1_655 ?
O77 Fe42 O76 87.5(13) . 1_655 ?
O79 Fe52 O78 94.7(14) . 1_455 ?
O79 Fe52 O81 95.0(16) . . ?
O78 Fe52 O81 91.9(14) 1_455 . ?
O79 Fe52 O80 172.8(15) . . ?
O78 Fe52 O80 87.1(13) 1_455 . ?
O81 Fe52 O80 91.9(14) . . ?
O79 Fe52 O83 87.6(15) . . ?
O78 Fe52 O83 101.7(14) 1_455 . ?
O81 Fe52 O83 165.9(14) . . ?
O80 Fe52 O83 85.2(13) . . ?
O79 Fe52 O82 90.5(14) . . ?
O78 Fe52 O82 174.7(13) 1_455 . ?
O81 Fe52 O82 86.5(14) . . ?
O80 Fe52 O82 87.9(13) . . ?
O83 Fe52 O82 79.6(13) . . ?
O84 Fe62 O85 99.3(14) . . ?
O84 Fe62 O86 88.0(17) . . ?
O85 Fe62 O86 94.8(16) . . ?
O84 Fe62 O88 89.4(14) . . ?
O85 Fe62 O88 170.1(15) . . ?
O86 Fe62 O88 90.3(16) . . ?
O84 Fe62 O87 92.5(14) . . ?
O85 Fe62 O87 92.2(15) . . ?
O86 Fe62 O87 172.9(16) . . ?
O88 Fe62 O87 82.6(14) . . ?
O84 Fe62 O89 169.7(12) . . ?
O85 Fe62 O89 88.5(13) . . ?
O86 Fe62 O89 98.0(16) . . ?
O88 Fe62 O89 82.3(13) . . ?
O87 Fe62 O89 80.5(12) . . ?
O90 Fe72 O92 96.0(14) . . ?
O90 Fe72 O73 98.7(14) . 1_545 ?
O92 Fe72 O73 93.4(12) . 1_545 ?
O90 Fe72 O93 96.2(15) . . ?
O92 Fe72 O93 167.1(14) . . ?
O73 Fe72 O93 88.8(13) 1_545 . ?
O90 Fe72 O94 83.4(14) . . ?
O92 Fe72 O94 87.4(13) . . ?
O73 Fe72 O94 177.6(13) 1_545 . ?
O93 Fe72 O94 90.0(13) . . ?
O90 Fe72 O95 174.1(14) . . ?
O92 Fe72 O95 84.1(14) . . ?
O73 Fe72 O95 87.1(14) 1_545 . ?
O93 Fe72 O95 83.4(14) . . ?
O94 Fe72 O95 90.8(13) . . ?
O96 Fe82 O97 95.1(13) . . ?
O96 Fe82 O98 96.2(12) . . ?
O97 Fe82 O98 100.0(14) . . ?
O96 Fe82 O99 172.9(14) . . ?
O97 Fe82 O99 89.3(16) . . ?
O98 Fe82 O99 88.4(15) . . ?
O96 Fe82 O100 87.0(15) . . ?
O97 Fe82 O100 165.5(16) . . ?
O98 Fe82 O100 94.0(15) . . ?
O99 Fe82 O100 87.4(17) . . ?
O96 Fe82 O101 92.3(12) . . ?
O97 Fe82 O101 80.4(14) . . ?
O98 Fe82 O101 171.4(13) . . ?
O99 Fe82 O101 83.0(15) . . ?
O100 Fe82 O101 85.2(15) . . ?
O92 P12 O55 111.1(19) . . ?
O92 P12 O97 107.7(18) . . ?
O55 P12 O97 99.6(18) . . ?
O92 P12 O86 120(2) . . ?
O55 P12 O86 112(2) . . ?
O97 P12 O86 104(2) . . ?
O98 P22 O78 113.8(19) . . ?
O98 P22 O84 110.0(19) . . ?
O78 P22 O84 113.0(18) . . ?
O98 P22 O75 105.0(19) . . ?
O78 P22 O75 107.6(19) . . ?
O84 P22 O75 106.8(18) . . ?
O91 P32 O58 104.6(19) . . ?
O91 P32 O81 109(2) . . ?
O58 P32 O81 111(2) . . ?
O91 P32 O67 112(2) . . ?
O58 P32 O67 114(2) . . ?
O81 P32 O67 106(2) . . ?
O90 P42 O62 110(2) . . ?
O90 P42 O85 102(2) . . ?
O62 P42 O85 111(2) . . ?
O90 P42 O72 111(2) . . ?
O62 P42 O72 107(2) . . ?
O85 P42 O72 117(2) . . ?
O96 P52 O68 112.8(17) . . ?
O96 P52 O56 106.4(19) . . ?
O68 P52 O56 106(2) . . ?
O96 P52 O57 109.8(18) . . ?
O68 P52 O57 108.7(19) . . ?
O56 P52 O57 113(2) . . ?
O73 P62 O79 110(2) . . ?
O73 P62 O64 109.4(19) . . ?
O79 P62 O64 102(2) . . ?
O73 P62 O102 111.9(18) . . ?
O79 P62 O102 111(2) . . ?
O64 P62 O102 111(2) . . ?
O104 S12 O103 103.6(19) . . ?
O104 S12 O89 111.9(19) . . ?
O103 S12 O89 105.2(17) . . ?
O104 S12 O105 107(2) . . ?
O103 S12 O105 110.1(19) . . ?
O89 S12 O105 118.4(18) . . ?
O106 S22 O107 110(2) . . ?
O106 S22 O108 110(2) . . ?
O107 S22 O108 115(2) . . ?
O106 S22 O59 105.5(19) . . ?
O107 S22 O59 109.7(19) . . ?
O108 S22 O59 106(2) . . ?
P12 O55 Fe32 142.4(18) . . ?
P52 O56 Fe12 149(3) . . ?
P52 O57 Fe22 138(2) . 1_565 ?
P32 O58 Fe12 142(2) . . ?
S22 O59 Fe12 142(2) . . ?
P42 O62 Fe22 149(2) . . ?
P62 O64 Fe22 137(2) . 1_565 ?
P32 O67 Fe32 141(3) . . ?
P52 O68 Fe32 138(2) . . ?
P42 O72 Fe42 135(2) . . ?
P62 O73 Fe72 145(2) . 1_565 ?
P22 O75 Fe42 136(2) . . ?
P22 O78 Fe52 146(2) . 1_655 ?
P62 O79 Fe52 145(2) . . ?
P32 O81 Fe52 136(2) . . ?
P22 O84 Fe62 150(2) . . ?
P42 O85 Fe62 157(2) . . ?
P12 O86 Fe62 143(3) . . ?
S12 O89 Fe62 140.2(18) . . ?
P42 O90 Fe72 142(2) . . ?
P32 O91 Fe42 148(2) . 1_455 ?
P12 O92 Fe72 141(2) . . ?
P52 O96 Fe82 150.4(18) . . ?
P12 O97 Fe82 142(2) . . ?
P22 O98 Fe82 138(2) . . ?
P62 O102 Fe12 147(2) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe11 O5 1.904(18) . ?
Fe11 O2 1.938(18) . ?
Fe11 O3 1.962(19) 1_445 ?
Fe11 O6 2.05(2) . ?
Fe11 O4 2.09(2) . ?
Fe11 O7 2.14(3) . ?
Fe21 O9 1.957(18) . ?
Fe21 O10 1.958(17) . ?
Fe21 O8 1.970(18) . ?
Fe21 O11 2.04(3) . ?
Fe21 O12 2.05(3) . ?
Fe21 O13 2.09(3) . ?
Fe31 O14 1.92(2) . ?
Fe31 O15 1.954(18) 1_655 ?
Fe31 O17 1.97(2) 1_665 ?
Fe31 O22 2.02(3) . ?
Fe31 O18 2.07(3) . ?
Fe31 O23 2.08(3) 1_665 ?
Fe41 O16 1.946(16) . ?
Fe41 O19 1.95(2) . ?
Fe41 O24 1.972(16) . ?
Fe41 O21 2.03(2) . ?
Fe41 O20 2.08(3) . ?
Fe41 O25 2.09(3) . ?
Fe51 O26 1.917(18) 1_665 ?
Fe51 O27 1.917(17) . ?
Fe51 O40 1.960(19) . ?
Fe51 O28 2.02(2) . ?
Fe51 O29 2.07(3) 1_665 ?
Fe51 O41 2.09(3) . ?
Fe61 O42 1.903(18) . ?
Fe61 O30 1.921(19) 1_545 ?
Fe61 O31 1.927(15) 1_545 ?
Fe61 O45 2.05(3) . ?
Fe61 O44 2.07(2) . ?
Fe61 O43 2.14(2) . ?
Fe71 O32 1.897(16) . ?
Fe71 O46 1.915(18) . ?
Fe71 O33 1.94(2) . ?
Fe71 O35 2.07(3) . ?
Fe71 O34 2.07(3) . ?
Fe71 O1 2.08(2) . ?
Fe81 O37 1.907(18) . ?
Fe81 O36 1.912(19) . ?
Fe81 O48 1.94(2) . ?
Fe81 O47 2.02(3) . ?
Fe81 O39 2.04(2) . ?
Fe81 O38 2.08(2) . ?
P11 O5 1.516(17) . ?
P11 O32 1.518(15) . ?
P11 O26 1.545(16) . ?
P11 O8 1.554(16) . ?
P21 O37 1.513(16) . ?
P21 O27 1.518(16) . ?
P21 O31 1.537(14) . ?
P21 O19 1.537(16) . ?
P31 O2 1.512(15) . ?
P31 O9 1.522(16) . ?
P31 O17 1.540(17) . ?
P31 O42 1.543(16) . ?
P41 O15 1.508(17) . ?
P41 O36 1.520(17) . ?
P41 O46 1.535(16) . ?
P41 O30 1.542(16) . ?
P51 O40 1.509(16) . ?
P51 O3 1.513(16) . ?
P51 O16 1.520(15) . ?
P51 O14 1.533(17) . ?
P61 O24 1.502(15) . ?
P61 O33 1.513(17) . ?
P61 O48 1.528(18) . ?
P61 O10 1.530(16) . ?
S11 O39 1.464(18) . ?
S11 O50 1.48(2) . ?
S11 O49 1.49(2) . ?
S11 O51 1.49(2) . ?
S21 O54 1.47(2) . ?
S21 O53 1.48(2) . ?
S21 O6 1.48(2) . ?
S21 O52 1.498(19) . ?
Fe12 O102 1.89(3) . ?
Fe12 O56 1.89(3) . ?
Fe12 O58 1.97(3) . ?
Fe12 O59 2.06(3) . ?
Fe12 O60 2.11(3) . ?
Fe12 O61 2.12(3) . ?
Fe22 O62 1.90(3) . ?
Fe22 O57 1.95(3) 1_545 ?
Fe22 O65 1.98(4) . ?
Fe22 O64 1.99(3) 1_545 ?
Fe22 O63 2.02(5) . ?
Fe22 O66 2.04(3) 1_545 ?
Fe32 O67 1.88(4) . ?
Fe32 O68 1.94(3) . ?
Fe32 O55 1.96(3) . ?
Fe32 O70 2.02(4) . ?
Fe32 O69 2.03(4) . ?
Fe32 O71 2.10(4) . ?
Fe42 O72 1.88(3) . ?
Fe42 O91 1.93(3) 1_655 ?
Fe42 O75 1.95(3) . ?
Fe42 O74 2.05(5) . ?
Fe42 O77 2.11(3) . ?
Fe42 O76 2.13(4) 1_655 ?
Fe52 O79 1.86(3) . ?
Fe52 O78 1.88(3) 1_455 ?
Fe52 O81 1.96(3) . ?
Fe52 O80 2.04(3) . ?
Fe52 O83 2.11(4) . ?
Fe52 O82 2.14(3) . ?
Fe62 O84 1.86(3) . ?
Fe62 O85 1.90(3) . ?
Fe62 O86 1.92(4) . ?
Fe62 O88 2.01(4) . ?
Fe62 O87 2.02(3) . ?
Fe62 O89 2.06(2) . ?
Fe72 O90 1.87(3) . ?
Fe72 O92 1.92(3) . ?
Fe72 O73 1.94(3) 1_545 ?
Fe72 O93 2.02(4) . ?
Fe72 O94 2.11(3) . ?
Fe72 O95 2.22(4) . ?
Fe82 O96 1.85(2) . ?
Fe82 O97 1.91(3) . ?
Fe82 O98 1.95(3) . ?
Fe82 O99 1.99(4) . ?
Fe82 O100 2.06(4) . ?
Fe82 O101 2.09(3) . ?
P12 O92 1.51(2) . ?
P12 O55 1.52(2) . ?
P12 O97 1.54(2) . ?
P12 O86 1.54(2) . ?
P22 O98 1.52(2) . ?
P22 O78 1.52(2) . ?
P22 O84 1.53(2) . ?
P22 O75 1.55(2) . ?
P32 O91 1.53(2) . ?
P32 O58 1.53(2) . ?
P32 O81 1.53(2) . ?
P32 O67 1.53(3) . ?
P42 O90 1.50(2) . ?
P42 O62 1.51(2) . ?
P42 O85 1.52(2) . ?
P42 O72 1.56(2) . ?
P52 O96 1.52(2) . ?
P52 O68 1.52(2) . ?
P52 O56 1.52(2) . ?
P52 O57 1.53(2) . ?
P62 O73 1.51(2) . ?
P62 O79 1.51(2) . ?
P62 O64 1.53(2) . ?
P62 O102 1.54(2) . ?
S12 O104 1.47(2) . ?
S12 O103 1.47(2) . ?
S12 O89 1.48(2) . ?
S12 O105 1.49(2) . ?
S22 O106 1.46(2) . ?
S22 O107 1.47(2) . ?
S22 O108 1.48(2) . ?
S22 O59 1.49(2) . ?
OW1A OW1B 1.38(6) . ?
OW3A OW3B 1.38(11) . ?
OW2A OW2B 1.45(6) . ?
